pharmaceuticals. Phenol formaldehyde resin (bakelite) have good heat resistance, dimensional stability as well as good resistance to most solvents. It also shows good dielectric properties. This material is typically used in molding applications, electrical, radio, televisions and automotive parts where their good dielectric properties are of use. Some other uses include: impregnating paper, varnishes, decorative laminates for wall coverings. Polytriazole polymers are produced from monomers which bear both an alkyne and azide functional group. The monomer units are linked to each other by the a 1,2,3-triazole group; which is produced by the 1,3-dipolar cycloaddition, also called the azide-alkyne Huisgen cycloaddition. These polymers can take on the form of a strong resin, or a gel. With oligopeptide monomers containing a terminal alkyne and terminal azide the resulting clicked peptide polymer will be biodegradable due to action of endopeptidases on the oligopeptide unit. Branched polymers A monomer with functionality of 3 or more will introduce branching in a polymer and will ultimately form a cross-linked macrostructure or network even at low fractional conversion. The point at which a tree-like topology transits to a network is known as the gel point because it is signalled by an abrupt change in viscosity. One of the earliest so-called thermosets is known as bakelite. It is not always water that is released in step-growth polymerization: in acyclic diene metathesis or ADMET dienes polymerize with loss of ethene. Kinetics The kinetics and rates of step-growth polymerization can be described using a polyesterification mechanism. The simple esterification is an acid-catalyzed process in which protonation of the acid is followed by interaction with the alcohol to produce an ester and water. However, there are a few assumptions needed with this kinetic model. The first assumption is water (or any other condensation product) is efficiently removed. Secondly, the functional group reactivities are independent of chain length. Finally, it is assumed that each step only involves one alcohol and one acid. This is a general rate law degree of polymerization for polyesterification where n= reaction order. Self-catalyzed Polyesterification If no acid catalyst is added, the reaction will still proceed because the acid can act as its own catalyst. The rate of condensation at any time t can then be derived from the rate of disappearance of -COOH groups and The second-order term arises from its use as a catalyst, and k is the rate constant. For a system with equivalent quantities